Micromeso draping modelling of noncrimp fabrics


 Bridget Mary Howard
 1 years ago
 Views:
Transcription
1 Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are widely used in the composite materials as a reinforcement part due to a combination of both high mechanical properties in main fibre directions and better handling compared to UD tapes. For prediction of mechanical response of composite parts in particular with high curvature it is important to consider the local orientations and gaps in textile structures obtained after draping. For this goal the simulations on the textile structure scale (mesoscale) are commonly used. In the present work the new approach for the modelling of the textile structures is proposed. In this approach the mechanical properties of the textile yarns are obtained from the microscale simulations of the glass roving. This allows to investigate the dependency to the fibre volume fraction (FVFr) of the roving. Although microscale modelling as the basis for textile simulations was used in [1], but only small micromodels without taking into account the crosssection change during the compaction was investigated. Latter can play a major role in forming processes like RTM. The representative volume element (RVE) of the structure should be generated without the interpenetrations, which is hardly possible for geometrical generation especially for the complex textile structures such as NCFs [2]. New method for the generating of the free of interpenetrations RVE based on the thermal expansion in transverse direction was proposed. The other aspect of the composite simulations is the prediction of the mechanical properties. Commonly used method where the textile geometry is subtracted from the matrix is causes bad quality mesh of the model or fails at all. For this reason the mesh superposition (MSP) [3, 4] technique is preferable for investigating of the stiffness behaviour. In present work this was implemented in LS Dyna. 2 Micromodelling of the roving Generally the roving can be described as a transverse isotropic material with axis of symmetry on the roving length axis. There are six main deformation modes: length tension and compaction, transverse tension and compaction, shear and torsion. In this work following assumptions are made:  compression stiffness in length direction as well as tension stiffness in transverse direction of the roving is negligible;  length stiffness of the roving has a linear dependency only on FVFr and may be calculated due to mixture rule like E E is a filament elastic modulus;, where is the FVFr and l f l E l f  there is no significant strain in transverse direction due to length deformation, so the poisson s ratio ; lt  fibrefibre friction is assumed to be constant. The constitutive law of the roving material in this case may be written as follows: x 1 E l f x y 1 Et tt Et y z tt Et 1 Et z xy 1 2Gtl xy yz 1 2Gtt yz G 1 2 xz tl xz This means that we need to define four constants that should depend nonlinear on the FVFr θ. 2.1 Used models For determination of the missing mechanical properties, quasistatic FE simulations on microscale were performed. Used models for different load cases are presented on the Figure 1. (1)
2 Fig.1: Roving models used for microsimulations: (a) transverse compaction, (b) torsion and (c) shear loading cases. The mechanical properties of the filaments were taken from the data sheet of the glass roving, which was used for manufacturing of the lenowoven NCFs. The diameter of one filament is 17m, density g cm, isotropic elastic modulus E f 82GPa with poisson s ratio. 2 f d f. Friction coefficient for fibrefibre contact was chosen to be.3. The filaments in the roving have some degree of misalignment due to the manufacturing processes of the textile and roving itself. In this work this effect was investigated by performing the simulations for various standard deviations of the filament angle. The structures were generated with GeoDict software [5] and then these models were transferred to LSDyna a converter software with developed in FTA [6]. These models have about 6 filaments inside of the domain of 1x.5x.5 mm³ for dom x, dom y and dom z respectively. Initial FVFr of the models was about 25% depending on the standard deviation of the filament orientations. To ensure the contact, each filament is represented as a sequence of HighLiu beams with length of l 2 d 34m. Rigid walls (RW) are generated on the sides of the domain. Periodicity in length f b f direction was implemented through restriction of displacement in xdirections as well as rotations along y and z axis for nodes, that lie on the domain x face. 2.2 Transverse compaction The general model for transverse compaction is represented at Figure 1 a. The roving is compressed in z direction so as the final FVFr would be. 85. f The upper RW z compresses the roving, while other three remain stationary. This approach allows to investigate on one loading case both the compression stiffness and the expansion effect in other transverse direction (y), which is nonlinear and may be significant for higher FVFrs. The pressure versus FVFr dependency for both z and y directions is shown in Figure 2. It may be seen, that the basic shape of the curves remains the same with shifting to small FVFr when the filament misalignment increases. Both y and z pressures start to increase at the same FVFr. f
3 Fig.2: Pressure in compression and transverse directions of the roving on microscale for different standard deviations of the filaments orientations. Further, the poisson s ratio and transverse elastic modulus may be expressed through the RW pressure values as follows: P P ; E P P, (2) tt y z t z tt y z where z is the logarithmic strain in compaction direction. Fig.3: Elastic modulus and poisson s coefficient of the roving on microscale for different standard deviations of the filaments orientations. The shape of the E comp curve remains smooth, while the poisson s tends to oscillate (Figure 3). It can be solved by using the models with higher amount of filaments inside and thus bigger domain dimansions. Still with used models the general trends of increasing of the poisson s ratio with increasing of the FVFr. The slope of the curve decreases with increasing of the filament misalignment. Model results were written out during the solution for FVFr of.5,.6,.7 and.8 for further torsion and shear calculations. 2.3 Torsion The torsion of 1 is applied to the roving as shown on the Figure 1 b. The shear modulus is then computed as follows: where inertia. G 2 E dom J int 2 x tt, (3) E int is the internal energy of the roving,  torsion angle and J is a polar area moment of
4 Results for different FVFr and filament misalignments with standard deviation of 1 and 4 are presented in the Figure 4. It may be seen, that with increasing of the FVFr and torsion angle the shear modulus in the ttplane increases. Fig.4: Shear modulus G tt versus torsion angle for a) 1 standard deviation of the filament orientation and b) Shear For the same models the shear simulations for determination of the shear modulus G lt were performed (Figure 1 c). Obtained shear modulus for standard deviation of 1 and 4 are represented in the Figure 5. Fig.5: Shear modulus G lt versus shear angle for a) 1 standard deviation of the filament orientation and b) 4. In this case it may be seen, that the shear modulus G lt doesn t change with the shear angle. As well as the trend to decreasing of the stiffness with increasing of the FVFr may be observed. This effect should be investigated in further studies. 3 Implementation of user defined material model The FVFr of the element may be obtained at each iteration as follows: exp, (4) t exp where is the initial FVFr of the element and 2 and 3 are the complete strains in the 2 and 3 directions respectively. The elastic modulus obtained from microscale simulation may be approximated with the power law as described in [1]. The poisson s ratio is also assumed to be approximated with power law. The shear modules are linear dependent from the FVFr: 2 3
5 B B E Et AE tt A ; Gtt At Bt ; Glt Al ; B, (5) where the A and B are constants for different mechanical properties obtained from the microsimulations of the roving. 4 Generation of the RVEs For the generation of the RVE the thermal expansion in the transverse direction of the rovings was used. It allows generating the complex textile structures without interpenetrations and use them for various simulations. The user defined material model described above was assigned to yarns. This allows to consider the local FVFr and real compression / shear behaviour. The dirichlet periodic boundary conditions (BC) were applied to the ends of the each yarn to estimate the periodicity of the obtained structure. Although the length of the auxiliary yarns was taken from the measurements on the real textile. Different RVE should be used for draping and mechanical simulations. From one hand, in the draping simulations the big areas of the textile should be modelled, so the model simplification plays very important role. The auxiliary yarns may be represented as beam elements and only two solid elements in thickness directions of the reinforcement yarns should be used. On the other hand, in mechanical simulations also the stress distributions inside of the auxiliary yarns and close to them may play a role, so more refined RVE is preferable. For this case the true shape of the yarns should be considered. 4.1 Draping simulation The initial textile structure with rescaled crosssections of the yarns is shown in the Figure 6. The auxiliary yarns in the initial condition have the circle crosssection and for preserving of the crosssection change during the thermal expansion simulation, the material MAT_22 was used with high transverse and length modules ( E1 E2 E3 ) but remaining the shear modules on the roving level. Different scale factors ( sf d init d real ) were used. l Fig.6: RVE of the lenowoven NCF for draping simulation: a) initial conditions, b) after thermal expansion simulation with calculated local FVFrs and c) auxiliary yarns are represented as beams. Obtained structure consists only of 112 solid elements and 6 beam elements with dimensions of RVE 4 x 4 cm². 4.2 Calculation of the mechanical properties In real structure the auxiliary yarns have an elliptical crosssection. This should be considered in the initial configuration, what yields to smaller initial crosssections. For obtaining the desired composite thickness, the rigid walls on the top and the bottom of the structure are generated (Figure 7).
6 Fig.7: RVE of the lenowoven NCF for calculation of the mechanical properties: a) initial conditions, b) after thermal expansion simulation with calculated local FVFrs. The crosssection of the generated structure conforms to the microcut image of real textile like shown in the Figure 8. Fig.8: Microcut image of the glass lenowoven NCF composite (a) and comparison with the simulation section view (b). 5 Validation of the developed model 5.1 Single roving compaction For validation purposes, the following experiment setup was used (Figure 9 a). It consists of two plates with the lower one is made of transparent material. A camera is located underneath, which is needed to record the width change during the compaction.
7 Fig.9: Roving compaction: a) experimental stand, b) roving outer surface. For estimation of the required parameters of the developed material model, the filament orientation distribution is necessary. For this purpose the outer surface of rovings taken from lenowoven NCF was microscopically investigated and the mean and standard deviation values were calculated (Figure 9 b). For this structure the average standard deviation value of the filament misalignment was The values of the transverse compaction elastic modulus and poisson s ratio were averaged between 5 and 6. The approximation with a power function is shown in Figure 1. Fig.1: Material parameters used for roving simulations: a) elastic modulus and b) poisson s ratio. The simulation results are showing good agreement with experimental results without some extra tuning of the parameters as it is shown on the Figure 11. Although some small deviations may be observed. These may be the reason of using relative small models for microsimulations as discussed above.
8 Fig.11: Comparison of the experimental and simulation results for roving compaction: a) compaction force per unit length and b) roving width versus roving thickness. 5.2 Stiffness of the composite The RVE described in Section 4.2 was used for prediction of the mechanical properties of the composite. For coupling of the textile reinforcement to the matrix the MSP technique was used. It was implemented in LSDyna by using of the *CONSTRAINED_MULTIPLE_GLOBAL keyword and placing the nodes of the textile mesh as first in the assignment. The same keyword was used to apply the dirichlet periodical BC to the matrix faces. Simulations for all six load cases with implicit iterative solver were performed and then homogenized mechanical properties were compared with experimental in the Table 1. Maximal error lies below 4%. Mechanical property Experiment Simulation Error E x, GPa 37,7 ±,55 36,72,7% E y, GPa 1,5 ±,2 1,9 3,8% G xy, GPa  3,7 µ xy,25,33 µ yx,87,1 Table 1: Mechanical properties of the composite based on lenowoven UD NCF. 5.3 Drapeability Described in Section 4.1 RVE of lenowoven NCF was used to perform the drapeability simulation (Figure 12). Due to the symmetry only one fourth of the model was built with the textile diameter of 33 mm.
9 Fig.12: Model for the draping simulation. In considered test, the punch drives until 8 mm into the fabric from underneath and at steps of 1 mm the force of the punch is taken as well as the pictures of textile on several positions. Total punch force calculated within simulation shows very good agreement with test results (Figure 13). Fig.13: Punch force versus punch displacement obtained from simulation and experiment. The pictures of the textile structure at the highest punch location are compared in the Figure 14. Both experiment and simulation are showing very small amount of gaps at and 45 whereas at 9 the DRAPETEST shows more local gaps which are not observed in simulation results.
10 c) d) e) f) Fig.14: Textile pictures taken from the DRAPETEST camera at the punch displacement 8 mm on a), b) 45 and c) 9 and at the corresponding positions from simulation d f. The contour of the textile after draping made with the camera on the top of the DRAPETEST has very good agreement with the simulation results (Figure 15). Fig.15: Textile shape after draping: a) DRAPETEST and b) simulation.
11 6 Summary In the present work a novel approach for modelling of the reinforcement NCFs was proposed. For estimating of the mechanical behaviour of the textile yarns the microscopic simulations of the roving with different levels of filament misalignments were performed. Obtained properties were direct transferred in the developed user material model and without any parameter tuning very good agreement with experimental results of simple roving compaction was reached both for compression force and crosssection shape change. This material model was also used for generating of the RVE using thermal expansion method of glass lenowoven NCF for different scales of refinement. The drapeability of the textile structure was validated based on drapeability tester called DRAPETEST by Textechno. The forming force converges very well with the measured experimentally. Also the deformation of the textile has the same character. This model may be useful also in simulations of other forming processes like RTM, where the crosssection changes may be significant. MSP method for calculation of the mechanical properties of textile reinforcement composite was implemented in LS Dyna. This method gave the error below 4% comparing to the experimental results. 7 Literature [1] Sherburn M., Geometric and Mechanical Modelling of Textiles, PhD thesis, 27 [2] Lomov S.V., Ivanov D.S., Verpoest I., Zako M., Kurashiki T., Nakai H., Hirosawa S., "MesoFE modelling of textile composites: Road map, data flow and algorithms," Composites Science and Technology, no. 67, pp , 27. [3] Tabatabaei S.A., Lomov S.V., Verpoest I., "Assesment of embedded element technique in mesofe modelling of fibre reinforced composites," Composite structures, no. 17, pp , 214. [4] Jiang WG, Hallett SR, Wisnom M., "Development of domain superposition technique for the modelling of woven fabric composites," in Mechanical response of composites.: Springer, 28. [5] [6] O. Vorobiov: "Interfacing GeoDict Analytical Data to LSDyna and ANSYS", GeoDict User Meeting 214, Kaiserslautern, 214
EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationMODELLING OF DAMAGE IN TEXTILE REINFORCED COMPOSITES: MICRO MESO APPROACH
B. Van Den Broucke et.al., Modelling of damage in textile reinforced composites: micro meso approach MODELLING OF DAMAGE IN TEXTILE REINFORCED COMPOSITES: MICRO MESO APPROACH B. Van Den Broucke,2,, P.
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationScienceDirect. Unit cell model of woven fabric textile composite for multiscale analysis. Anurag Dixit a *,Harlal Singh Mali b, R.K.
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 68 ( 2013 ) 352 358 The Malaysian International Tribology Conference 2013 (MITC2013) Unit cell model of woven fabric textile
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationUnit 15 Shearing and Torsion (and Bending) of Shell Beams
Unit 15 Shearing and Torsion (and Bending) of Shell Beams Readings: Rivello Ch. 9, section 8.7 (again), section 7.6 T & G 126, 127 Paul A. Lagace, Ph.D. Professor of Aeronautics & Astronautics and Engineering
More informationINDUSTRIAL FORMING SIMULATION OF MULTILAYERED UD NONCRIMPFABRICS. 13. LSDYNA FORUM, , BAMBERG.
Sebastian Kreissl, Thomas Senner, Arnulf Lipp, Josef Meinhardt. INDUSTRIAL FORMING SIMULATION OF MULTILAYERED UD NONCRIMPFABRICS. 13. LSDYNA FORUM, 07.10.2014, BAMBERG. OUTLINE. BMW i. Production Process
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationPLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile
More informationInsitu local strain measurement in textile composites with embedded optical fibre sensors
Insitu local strain measurement in textile composites with embedded optical fibre sensors S. Daggumati, E. Voet, I. De Baere, W. Van Paepegem & J. Degrieck Ghent University, Department of Materials Science
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationEXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationReview of Strain Energy Methods and Introduction to Stiffness Matrix Methods of Structural Analysis
uke University epartment of Civil and Environmental Engineering CEE 42L. Matrix Structural Analysis Henri P. Gavin Fall, 22 Review of Strain Energy Methods and Introduction to Stiffness Matrix Methods
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationContent. Department of Mathematics University of Oslo
Chapter: 1 MEK4560 The Finite Element Method in Solid Mechanics II (January 25, 2008) (Epost:torgeiru@math.uio.no) Page 1 of 14 Content 1 Introduction to MEK4560 3 1.1 Minimum Potential energy..............................
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More information3. Overview of MSC/NASTRAN
3. Overview of MSC/NASTRAN MSC/NASTRAN is a general purpose finite element analysis program used in the field of static, dynamic, nonlinear, thermal, and optimization and is a FORTRAN program containing
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationCOMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS. Abstract. Introduction
COMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS HsiangChuan Tsai, National Taiwan University of Science and Technology, Taipei, Taiwan James M. Kelly, University of California,
More informationY. M. TEMIS AND V. V. KARABAN 1
J. KSIAM Vol.5, No.2, 3951, 2001 BOUNDARY ELEMENT TECHNIQUE IN TORSION PROBLEMS OF BEAMS WITH MULTIPLY CONNECTED CROSSSECTIONS Y. M. TEMIS AND V. V. KARABAN 1 Abstract. This paper shows how boundary
More informationIraq Ref. & Air. Cond. Dept/ Technical College / Kirkuk
International Journal of Scientific & Engineering Research, Volume 6, Issue 4, April015 1678 Study the Increasing of the Cantilever Plate Stiffness by Using s Jawdat Ali Yakoob Iesam Jondi Hasan Ass.
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationModule 10: Free Vibration of an Undampened 1D Cantilever Beam
Module 10: Free Vibration of an Undampened 1D Cantilever Beam Table of Contents Page Number Problem Description Theory Geometry 4 Preprocessor 6 Element Type 6 Real Constants and Material Properties 7
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationMECHANICAL BEHAVIOR OF WOVEN FABRIC COMPOSITES UNDER MESOLEVEL UNCERTAINTIES: MODELING AND SENSITIVITY ANALYSIS. Mojtaba Komeili
MECHANICAL BEHAVIOR OF WOVEN FABRIC COMPOSITES UNDER MESOLEVEL UNCERTAINTIES: MODELING AND SENSITIVITY ANALYSIS by Mojtaba Komeili B.Sc. Iran University of Science and Technology, Iran, 2008 A THESIS
More informationINFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS
ISSN 18466168 (Print), ISSN 18485588 (Online) ID: TG217816142553 Original scientific paper INFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS Željko PENAVA, Diana ŠIMIĆ PENAVA, Željko
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationMechanics of Irregular Honeycomb Structures
Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationA Suggested Analytical Solution for Vibration of Honeycombs Sandwich Combined Plate Structure
International Journal of Mechanical & Mechatronics Engineering IJMMEIJENS Vol:16 No:04 9 A Suggested Analytical Solution for Vibration of Honeycombs Sandwich Combined Plate Structure Muhsin J. Jweeg College
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More informationAnalysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements
Acta Mech. Sin. (2016) 32(2):295 300 DOI 10.1007/s1040901505342 RESEARCH PAPER Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements V. H. Carneiro 1
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationFinite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras. Module  01 Lecture  11
Finite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras Module  01 Lecture  11 Last class, what we did is, we looked at a method called superposition
More informationChapter 12. Static Equilibrium and Elasticity
Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial
More informationGame Physics. Game and Media Technology Master Program  Utrecht University. Dr. Nicolas Pronost
Game and Media Technology Master Program  Utrecht University Dr. Nicolas Pronost Soft body physics Soft bodies In reality, objects are not purely rigid for some it is a good approximation but if you hit
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationSymmetric Bending of Beams
Symmetric Bending of Beams beam is any long structural member on which loads act perpendicular to the longitudinal axis. Learning objectives Understand the theory, its limitations and its applications
More informationNonlinear Analysis of Reinforced Concrete Shells Subjected to Impact Loads
Transactions of the 7 th International Conference on Structural Mechanics in Reactor Technology (SMiRT 7) Prague, Czech Republic, August 7, 00 Paper # J0 Nonlinear Analysis of Reinforced Concrete Shells
More informationFeatures and design of elastomer / textile engineered structures. D Boast, C Eng. F Mech E.
Features and design of elastomer / textile engineered structures D Boast, C Eng. F Mech E. Title of meeting IOM Bla blah Topics Materials: Environmental acids, water, oil, radiation etc. Bonding. Cost.
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationStresses and Strains in flexible Pavements
Stresses and Strains in flexible Pavements Multi Layered Elastic System Assumptions in Multi Layered Elastic Systems The material properties of each layer are homogeneous property at point A i is the same
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationBridge deck modelling and design process for bridges
EURussia Regulatory Dialogue Construction Sector Subgroup 1 Bridge deck modelling and design process for bridges Application to a composite twingirder bridge according to Eurocode 4 Laurence Davaine
More informationSimulation Analysis of Microchannel Deformation during LTCC Warm Water Isostatic Pressing Process Lang Ping, Zhaohua Wu*
International Conference on Information Sciences, Machinery, Materials and Energy (ICISMME 2015) Simulation Analysis of Microchannel Deformation during LTCC Warm Water Isostatic Pressing Process Lang Ping,
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationPHYSICS. Course Structure. Unit Topics Marks. Physical World and Measurement. 1 Physical World. 2 Units and Measurements.
PHYSICS Course Structure Unit Topics Marks I Physical World and Measurement 1 Physical World 2 Units and Measurements II Kinematics 3 Motion in a Straight Line 23 4 Motion in a Plane III Laws of Motion
More informationSERVICEABILITY OF BEAMS AND ONEWAY SLABS
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition Fifth Edition SERVICEABILITY OF BEAMS AND ONEWAY SLABS A. J. Clark School of Engineering Department of Civil
More informationLateral Crushing of Square and Rectangular Metallic Tubes under Different QuasiStatic Conditions
Vol:, No:1, 2 Lateral Crushing of Square and Rectangular Metallic Tubes under Different QuasiStatic Conditions Sajjad Dehghanpour, Ali Yousefi International Science Index, Mechanical and Mechatronics
More informationModule 4 : Deflection of Structures Lecture 4 : Strain Energy Method
Module 4 : Deflection of Structures Lecture 4 : Strain Energy Method Objectives In this course you will learn the following Deflection by strain energy method. Evaluation of strain energy in member under
More informationIf the number of unknown reaction components are equal to the number of equations, the structure is known as statically determinate.
1 of 6 EQUILIBRIUM OF A RIGID BODY AND ANALYSIS OF ETRUCTURAS II 9.1 reactions in supports and joints of a twodimensional structure and statically indeterminate reactions: Statically indeterminate structures
More informationFinite Element Method (FEM)
Finite Element Method (FEM) The finite element method (FEM) is the oldest numerical technique applied to engineering problems. FEM itself is not rigorous, but when combined with integral equation techniques
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationNew Representation of Bearings in LSDYNA
13 th International LSDYNA Users Conference Session: Aerospace New Representation of Bearings in LSDYNA Kelly S. Carney Samuel A. Howard NASA Glenn Research Center, Cleveland, OH 44135 Brad A. Miller
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationTRESS  STRAIN RELATIONS
TRESS  STRAIN RELATIONS Stress Strain Relations: Hook's law, states that within the elastic limits the stress is proportional to t is impossible to describe the entire stress strain curve with simple
More informationWe are IntechOpen, the first native scientific publisher of Open Access books. International authors and editors. Our authors are among the TOP 1%
We are IntechOpen, the first native scientific publisher of Open Access books 3,350 108,000 1.7 M Open access books available International authors and editors Downloads Our authors are among the 151 Countries
More informationEsben Byskov. Elementary Continuum. Mechanics for Everyone. With Applications to Structural Mechanics. Springer
Esben Byskov Elementary Continuum Mechanics for Everyone With Applications to Structural Mechanics Springer Contents Preface v Contents ix Introduction What Is Continuum Mechanics? "I Need Continuum Mechanics
More informationSound Propagation through Media. Nachiketa Tiwari Indian Institute of Technology Kanpur
Sound Propagation through Media Nachiketa Tiwari Indian Institute of Technology Kanpur LECTURE13 WAVE PROPAGATION IN SOLIDS Longitudinal Vibrations In Thin Plates Unlike 3D solids, thin plates have surfaces
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationMarch 24, Chapter 4. Deflection and Stiffness. Dr. Mohammad Suliman Abuhaiba, PE
Chapter 4 Deflection and Stiffness 1 2 Chapter Outline Spring Rates Tension, Compression, and Torsion Deflection Due to Bending Beam Deflection Methods Beam Deflections by Superposition Strain Energy Castigliano
More informationC:\Users\whit\Desktop\Active\304_2012_ver_2\_Notes\4_Torsion\1_torsion.docx 6
C:\Users\whit\Desktop\Active\304_2012_ver_2\_Notes\4_Torsion\1_torsion.doc 6 p. 1 of Torsion of circular bar The crosssections rotate without deformation. The deformation that does occur results from
More information14. LSDYNA Forum 2016
14. LSDYNA Forum 2016 A Novel Approach to Model Laminated Glass R. Böhm, A. Haufe, A. Erhart DYNAmore GmbH Stuttgart 1 Content Introduction and Motivation Common approach to model laminated glass New
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More information14. *14.8 CASTIGLIANO S THEOREM
*14.8 CASTIGLIANO S THEOREM Consider a body of arbitrary shape subjected to a series of n forces P 1, P 2, P n. Since external work done by forces is equal to internal strain energy stored in body, by
More informationChapter 5. Vibration Analysis. Workbench  Mechanical Introduction ANSYS, Inc. Proprietary 2009 ANSYS, Inc. All rights reserved.
Workbench  Mechanical Introduction 12.0 Chapter 5 Vibration Analysis 51 Chapter Overview In this chapter, performing free vibration analyses in Simulation will be covered. In Simulation, performing a
More informationU.S. South America Workshop. Mechanics and Advanced Materials Research and Education. Rio de Janeiro, Brazil. August 2 6, Steven L.
Computational Modeling of Composite and Functionally Graded Materials U.S. South America Workshop Mechanics and Advanced Materials Research and Education Rio de Janeiro, Brazil August 2 6, 2002 Steven
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationCrash Safety of LithiumIon Batteries for Electric Vehicles
Crash Safety of LithiumIon Batteries for Electric Vehicles Elham Sahraei Esfahani Research Scientist, MIT Assistant Professor, GMU Vehicle Crashes and Testing Battery Packs in T Configuration Chevy Volt
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationPlane and axisymmetric models in Mentat & MARC. Tutorial with some Background
Plane and axisymmetric models in Mentat & MARC Tutorial with some Background Eindhoven University of Technology Department of Mechanical Engineering Piet J.G. Schreurs Lambèrt C.A. van Breemen March 6,
More informationJeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA UNESCO EOLSS
MECHANICS OF MATERIALS Jeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA Keywords: Solid mechanics, stress, strain, yield strength Contents 1. Introduction 2. Stress
More informationExperimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 pebbles
Experimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 s D. Aquaro 1 N. Zaccari ABSTRACT Dipartimento di Ingegneria Meccanica Nucleare e della Produzione University of Pisa (Italy)
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationIntroduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams.
Outline of Continuous Systems. Introduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams. Vibrations of Flexible Strings. Torsional Vibration of Rods. BernoulliEuler Beams.
More informationMODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE
8th International DAAAM Baltic Conference INDUSTRIAL ENGINEERING 1921 April 2012, Tallinn, Estonia MODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE Pabut, O.; Allikas, G.; Herranen,
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationEE C247B / ME C218 INTRODUCTION TO MEMS DESIGN SPRING 2014 C. Nguyen PROBLEM SET #4
Issued: Wednesday, Mar. 5, 2014 PROBLEM SET #4 Due (at 9 a.m.): Tuesday Mar. 18, 2014, in the EE C247B HW box near 125 Cory. 1. Suppose you would like to fabricate the suspended cross beam structure below
More informationEE C245 ME C218 Introduction to MEMS Design
EE C245 ME C218 Introduction to MEMS Design Fall 2007 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture 16: Energy
More informationELASTICITY (MDM 10203)
LASTICITY (MDM 10203) Lecture Module 5: 3D Constitutive Relations Dr. Waluyo Adi Siswanto University Tun Hussein Onn Malaysia Generalised Hooke's Law In one dimensional system: = (basic Hooke's law) Considering
More informationVirtual distortions applied to structural modelling and sensitivity analysis. Damage identification testing example
AMAS Workshop on Smart Materials and Structures SMART 03 (pp.313 324) Jadwisin, September 25, 2003 Virtual distortions applied to structural modelling and sensitivity analysis. Damage identification testing
More informationMODELLING OF THE RIVET FORMING PROCESS IN ALUMINUM AND GLARE FOR DESIGN AGAINST FATIGUE
MODELLING OF THE RIVET FORMING PROCESS IN ALUMINUM AND GLARE FOR DESIGN AGAINST FATIGUE Calvin D. Rans 1, René C. Alderliesten 2, Paul V. Straznicky 1 1 Department of Mechanical and Aerospace Engineering,
More informationFinite Element Modelling with Plastic Hinges
01/02/2016 Marco Donà Finite Element Modelling with Plastic Hinges 1 Plastic hinge approach A plastic hinge represents a concentrated postyield behaviour in one or more degrees of freedom. Hinges only
More informationChapter 3 LAMINATED MODEL DERIVATION
17 Chapter 3 LAMINATED MODEL DERIVATION 3.1 Fundamental Poisson Equation The simplest version of the frictionless laminated model was originally introduced in 1961 by Salamon, and more recently explored
More informationSTATICALLY INDETERMINATE STRUCTURES
STATICALLY INDETERMINATE STRUCTURES INTRODUCTION Generally the trusses are supported on (i) a hinged support and (ii) a roller support. The reaction components of a hinged support are two (in horizontal
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 1
MECE 3321 MECHANICS O SOLIDS CHAPTER 1 Samantha Ramirez, MSE WHAT IS MECHANICS O MATERIALS? Rigid Bodies Statics Dynamics Mechanics Deformable Bodies Solids/Mech. Of Materials luids 1 WHAT IS MECHANICS
More informationFINITE ELEMENT ANALYSIS OF THE ELASTIC CONSTITUTIVE BEHAVIOR OF A 2.5D INTERLOCK COMPOSITE
FINITE ELEMENT ANALYSIS OF THE ELASTIC CONSTITUTIVE BEHAVIOR OF A 2.5D INTERLOCK COMPOSITE NEHME Samer *, HAGEGE Benjamin *, KAABI Abderrahmen **, BENZEGGAGH Malk * * Université de Technologie de Compiègne,
More informationFinite elementbased elastoplastic optimum reinforcement dimensioning of spatial concrete panel structures
Research Collection Report Finite elementbased elastoplastic optimum reinforcement dimensioning of spatial concrete panel structures Author(s): Tabatabai, Seyed Mohammad Reza Publication Date: 1996 Permanent
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More information